 
data_1 
 
_audit_creation_method            SHELXL-97 
_chemical_name_systematic 
; 
 ? 
; 
_chemical_name_common             ? 
_chemical_melting_point           ? 
_chemical_formula_moiety          ? 
_chemical_formula_sum 
 'B11 Ba2 H7 O22' 
_chemical_formula_weight          752.65 
 
loop_ 
 _atom_type_symbol 
 _atom_type_description 
 _atom_type_scat_dispersion_real 
 _atom_type_scat_dispersion_imag 
 _atom_type_scat_source 
 'B'  'B'   0.0013   0.0007 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'H'  'H'   0.0000   0.0000 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'O'  'O'   0.0106   0.0060 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Ba'  'Ba'  -0.3244   2.2819 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 
_symmetry_cell_setting            triclinic 
_symmetry_space_group_name_H-M    P-1 
 
loop_ 
 _symmetry_equiv_pos_as_xyz 
 'x, y, z' 
 '-x, -y, -z' 
 
_cell_length_a                    6.7745(11) 
_cell_length_b                    6.8452(16) 
_cell_length_c                    21.531(4) 
_cell_angle_alpha                 88.152(16) 
_cell_angle_beta                  82.974(12) 
_cell_angle_gamma                 60.518(9) 
_cell_volume                      862.2(3) 
_cell_formula_units_Z             2 
_cell_measurement_temperature     296(2) 
_cell_measurement_reflns_used     4395 
_cell_measurement_theta_min       0.95 
_cell_measurement_theta_max       27.54 
 
_exptl_crystal_description        'lamellar' 
_exptl_crystal_colour             'colourless' 
_exptl_crystal_size_max           0.15 
_exptl_crystal_size_mid           0.06 
_exptl_crystal_size_min           0.05 
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_diffrn     2.899 
_exptl_crystal_density_method     'not measured' 
_exptl_crystal_F_000              700 
_exptl_absorpt_coefficient_mu     4.661 
_exptl_absorpt_correction_type    empirical 
_exptl_absorpt_correction_T_min   0.5415 
_exptl_absorpt_correction_T_max   0.8004 
_exptl_absorpt_process_details    'SADABS (Sheldrick, 1996)' 
 
_exptl_special_details 
; 
 ? 
; 
 
_diffrn_ambient_temperature       296(2) 
_diffrn_radiation_wavelength      0.71073 
_diffrn_radiation_type            MoK\a 
_diffrn_radiation_source          'fine-focus sealed tube' 
_diffrn_radiation_monochromator   graphite 
_diffrn_measurement_device_type   'Bruker APEX-II area-detector diffractometer' 
_diffrn_measurement_method        'phi and omega scans'
_diffrn_detector_area_resol_mean  ? 
_diffrn_standards_number          none 
_diffrn_standards_interval_count  none 
_diffrn_standards_interval_time   none 
_diffrn_standards_decay_%         none 
_diffrn_reflns_number             12671 
_diffrn_reflns_av_R_equivalents   0.0356 
_diffrn_reflns_av_sigmaI/netI     0.0390 
_diffrn_reflns_limit_h_min        -8 
_diffrn_reflns_limit_h_max        8 
_diffrn_reflns_limit_k_min        -8 
_diffrn_reflns_limit_k_max        8 
_diffrn_reflns_limit_l_min        -27 
_diffrn_reflns_limit_l_max        27 
_diffrn_reflns_theta_min          0.95 
_diffrn_reflns_theta_max          27.54 
_reflns_number_total              3901 
_reflns_number_gt                 3253 
_reflns_threshold_expression      >2sigma(I) 
 
_computing_data_collection        'APEXII (Bruker, 2006)' 
_computing_cell_refinement        'SAINT (Bruker, 2006)'
_computing_data_reduction         'SAINT'
_computing_structure_solution     'SHELXS-97 (Sheldrick, 1990)' 
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)' 
_computing_molecular_graphics     'DIAMOND (Brandenburg, 1999)' 
_computing_publication_material   'SHELXTL (Sheldrick, 2008)' 
 
_refine_special_details 
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
; 
 
_refine_ls_structure_factor_coef  Fsqd  
_refine_ls_matrix_type            full 
_refine_ls_weighting_scheme       calc  
_refine_ls_weighting_details 
 'calc w=1/[σ²(Fo²)+(0.0304P)²+0.0000P] where P=(Fo²+2Fc²)/3' 
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap 
_atom_sites_solution_hydrogens    geom 
_refine_ls_hydrogen_treatment     mixed 
_refine_ls_extinction_method      none 
_refine_ls_extinction_coef        ? 
_refine_ls_number_reflns          3901 
_refine_ls_number_parameters      337 
_refine_ls_number_restraints      14 
_refine_ls_R_factor_all           0.0364 
_refine_ls_R_factor_gt            0.0261 
_refine_ls_wR_factor_ref          0.0604 
_refine_ls_wR_factor_gt           0.0554 
_refine_ls_goodness_of_fit_ref    1.025 
_refine_ls_restrained_S_all       1.033 
_refine_ls_shift/su_max           0.003 
_refine_ls_shift/su_mean          0.000 
 
loop_ 
 _atom_site_label 
 _atom_site_type_symbol 
 _atom_site_fract_x 
 _atom_site_fract_y 
 _atom_site_fract_z 
 _atom_site_U_iso_or_equiv 
 _atom_site_adp_type 
 _atom_site_occupancy 
 _atom_site_symmetry_multiplicity 
 _atom_site_calc_flag 
 _atom_site_refinement_flags 
 _atom_site_disorder_assembly 
 _atom_site_disorder_group 
Ba1 Ba 0.30145(4) 0.35509(3) 0.057806(11) 0.01021(7) Uani 1 1 d . . . 
Ba2 Ba 0.34897(4) 0.84453(4) 0.447088(11) 0.01056(7) Uani 1 1 d . . . 
B1 B 0.2194(10) 0.3454(9) 0.2155(3) 0.0221(11) Uani 1 1 d . . . 
B2 B 0.6110(8) 0.6877(7) 0.0904(2) 0.0109(9) Uani 1 1 d . . . 
B3 B 0.6491(9) 0.5094(8) 0.1922(2) 0.0172(11) Uani 1 1 d . . . 
B4 B 0.7925(8) 0.2660(7) 0.0957(2) 0.0117(9) Uani 1 1 d . . . 
B5 B 1.1896(8) -0.0542(7) 0.0709(2) 0.0114(9) Uani 1 1 d . . . 
B6 B 0.8719(8) -0.1270(7) 0.0760(2) 0.0111(9) Uani 1 1 d . . . 
B7 B 0.8773(8) 0.4307(7) 0.4260(2) 0.0095(9) Uani 1 1 d . . . 
B8 B 1.2683(8) 0.3567(7) 0.4211(2) 0.0093(9) Uani 1 1 d . . . 
B9 B 0.9546(8) 0.7471(7) 0.4035(2) 0.0106(9) Uani 1 1 d . . . 
B10 B 0.8694(9) 0.9573(7) 0.3057(2) 0.0168(10) Uani 1 1 d . . . 
B11 B 0.7169(8) 1.1672(7) 0.4054(2) 0.0094(9) Uani 1 1 d . . . 
OW1 O 0.3616(9) 0.9139(6) 0.32651(16) 0.0507(13) Uani 1 1 d D . . 
HW1 H 0.309(12) 1.038(4) 0.309(2) 0.076 Uiso 1 1 d D . . 
HW2 H 0.433(11) 0.812(6) 0.2987(19) 0.076 Uiso 1 1 d D . . 
O1 O 0.1391(7) 0.5343(6) 0.18250(17) 0.0332(8) Uani 1 1 d DU . . 
H1 H 0.095(10) 0.657(5) 0.203(2) 0.050 Uiso 1 1 d D . . 
O2 O 0.1995(8) 0.3391(5) 0.27873(17) 0.0442(11) Uani 1 1 d D . . 
H2 H 0.137(11) 0.464(6) 0.300(3) 0.066 Uiso 1 1 d D . . 
O3 O 0.3268(7) 0.1584(5) 0.17780(15) 0.0295(8) Uani 1 1 d D . . 
H3 H 0.373(10) 0.028(4) 0.193(2) 0.044 Uiso 1 1 d D . . 
O4 O 0.6523(5) 0.4722(4) 0.06513(12) 0.0097(6) Uani 1 1 d . . . 
O5 O 0.4177(5) 0.8764(4) 0.06219(13) 0.0104(6) Uani 1 1 d . . . 
O6 O 0.5686(5) 0.7019(4) 0.15858(13) 0.0154(6) Uani 1 1 d . . . 
O7 O 0.6116(7) 0.5363(5) 0.25598(14) 0.0312(9) Uani 1 1 d D . . 
H7 H 0.663(10) 0.418(6) 0.277(2) 0.047 Uiso 1 1 d D . . 
O8 O 0.7600(5) 0.3006(4) 0.16434(13) 0.0158(6) Uani 1 1 d . . . 
O9 O 1.0381(5) 0.1702(4) 0.07252(13) 0.0131(6) Uani 1 1 d . . . 
O10 O 1.1082(5) -0.2024(4) 0.07391(14) 0.0155(6) Uani 1 1 d . . . 
O11 O 0.8205(5) -0.2920(4) 0.06799(13) 0.0113(6) Uani 1 1 d . . . 
O12 O 0.7254(5) 0.0958(4) 0.08186(13) 0.0126(6) Uani 1 1 d . . . 
O13 O 1.1071(5) 0.2813(4) 0.42215(13) 0.0122(6) Uani 1 1 d . . . 
O14 O 1.4844(5) 0.1932(4) 0.42822(13) 0.0104(6) Uani 1 1 d . . . 
O15 O 1.1926(5) 0.5790(4) 0.41710(13) 0.0112(6) Uani 1 1 d . . . 
O16 O 0.9570(6) 0.7575(4) 0.33589(13) 0.0175(7) Uani 1 1 d . . . 
O17 O 0.9015(7) 0.9400(5) 0.24184(14) 0.0309(9) Uani 1 1 d D . . 
H17 H 0.846(10) 1.072(4) 0.229(3) 0.046 Uiso 1 1 d D . . 
O18 O 0.7556(5) 1.1604(4) 0.33750(13) 0.0140(6) Uani 1 1 d . . . 
O19 O 0.7156(5) 1.3659(4) 0.43216(13) 0.0110(6) Uani 1 1 d . . . 
O20 O 0.8863(5) 0.9608(4) 0.43296(12) 0.0101(6) Uani 1 1 d . . . 
O21 O 0.8018(5) 0.6563(4) 0.42930(14) 0.0136(6) Uani 1 1 d . . . 
 
 
_geom_special_details 
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
; 
 
loop_ 
 _geom_bond_atom_site_label_1 
 _geom_bond_atom_site_label_2 
 _geom_bond_distance 
 _geom_bond_site_symmetry_2 
 _geom_bond_publ_flag 
Ba1 O9 2.635(3) 1_455 ? 
Ba1 O12 2.637(3) . ? 
Ba1 O10 2.657(3) 1_465 ? 
Ba1 O1 2.843(4) . ? 
Ba1 O3 2.859(3) . ? 
Ba1 O4 2.880(3) . ? 
Ba1 O4 2.909(3) 2_665 ? 
Ba1 O11 2.934(3) 1_465 ? 
Ba1 O5 2.970(2) 1_545 ? 
Ba1 O5 2.983(3) 2_665 ? 
Ba1 O11 3.030(3) 2_655 ? 
Ba1 B2 3.169(5) 2_665 ? 
Ba2 OW1 2.623(3) . ? 
Ba2 O15 2.642(3) 1_455 ? 
Ba2 O21 2.659(3) . ? 
Ba2 O13 2.684(2) 1_465 ? 
Ba2 O20 2.848(3) 2_676 ? 
Ba2 O20 2.883(3) 1_455 ? 
Ba2 O14 2.950(2) 1_465 ? 
Ba2 O19 2.978(3) 1_545 ? 
Ba2 O14 2.993(3) 2_766 ? 
Ba2 O19 3.021(3) 2_676 ? 
Ba2 B11 3.158(5) 2_676 ? 
Ba2 B7 3.278(5) . ? 
B1 O1 1.348(6) . ? 
B1 O2 1.352(6) . ? 
B1 O3 1.354(6) . ? 
B2 O6 1.458(5) . ? 
B2 O4 1.469(5) . ? 
B2 O5 1.494(5) . ? 
B2 O11 1.513(5) 1_565 ? 
B2 Ba1 3.169(5) 2_665 ? 
B3 O8 1.362(6) . ? 
B3 O7 1.367(6) . ? 
B3 O6 1.373(5) . ? 
B4 O4 1.450(5) . ? 
B4 O8 1.477(6) . ? 
B4 O9 1.481(5) . ? 
B4 O12 1.493(5) . ? 
B5 O9 1.363(5) . ? 
B5 O5 1.364(5) 1_645 ? 
B5 O10 1.369(5) . ? 
B5 Ba1 3.239(4) 1_655 ? 
B6 O12 1.349(5) . ? 
B6 O11 1.357(5) . ? 
B6 O10 1.415(5) . ? 
B6 Ba1 3.293(5) 1_645 ? 
B7 O19 1.361(5) 1_545 ? 
B7 O21 1.368(5) . ? 
B7 O13 1.372(5) . ? 
B8 O15 1.350(5) . ? 
B8 O14 1.360(5) . ? 
B8 O13 1.416(5) . ? 
B8 Ba2 3.311(4) 1_645 ? 
B9 O20 1.442(5) . ? 
B9 O16 1.453(5) . ? 
B9 O21 1.496(5) . ? 
B9 O15 1.509(5) . ? 
B9 Ba2 3.298(4) 1_655 ? 
B10 O17 1.364(6) . ? 
B10 O18 1.369(6) . ? 
B10 O16 1.373(5) . ? 
B11 O18 1.451(5) . ? 
B11 O20 1.478(5) . ? 
B11 O19 1.490(5) . ? 
B11 O14 1.515(5) 1_465 ? 
B11 Ba2 3.158(5) 2_676 ? 
OW1 HW1 0.837(10) . ? 
OW1 HW2 0.839(10) . ? 
O1 H1 0.856(10) . ? 
O2 H2 0.856(10) . ? 
O3 H3 0.852(10) . ? 
O4 Ba1 2.909(3) 2_665 ? 
O5 B5 1.364(5) 1_465 ? 
O5 Ba1 2.970(2) 1_565 ? 
O5 Ba1 2.983(3) 2_665 ? 
O7 H7 0.848(10) . ? 
O9 Ba1 2.635(3) 1_655 ? 
O10 Ba1 2.657(3) 1_645 ? 
O11 B2 1.513(5) 1_545 ? 
O11 Ba1 2.934(3) 1_645 ? 
O11 Ba1 3.030(3) 2_655 ? 
O13 Ba2 2.684(2) 1_645 ? 
O14 B11 1.515(5) 1_645 ? 
O14 Ba2 2.950(2) 1_645 ? 
O14 Ba2 2.993(3) 2_766 ? 
O15 Ba2 2.642(3) 1_655 ? 
O17 H17 0.844(10) . ? 
O19 B7 1.361(5) 1_565 ? 
O19 Ba2 2.978(3) 1_565 ? 
O19 Ba2 3.021(3) 2_676 ? 
O20 Ba2 2.848(3) 2_676 ? 
O20 Ba2 2.883(3) 1_655 ? 
 
loop_ 
 _geom_angle_atom_site_label_1 
 _geom_angle_atom_site_label_2 
 _geom_angle_atom_site_label_3 
 _geom_angle 
 _geom_angle_site_symmetry_1 
 _geom_angle_site_symmetry_3 
 _geom_angle_publ_flag 
O9 Ba1 O12 115.44(8) 1_455 . ? 
O9 Ba1 O10 118.51(9) 1_455 1_465 ? 
O12 Ba1 O10 119.60(8) . 1_465 ? 
O9 Ba1 O1 88.91(10) 1_455 . ? 
O12 Ba1 O1 93.90(10) . . ? 
O10 Ba1 O1 62.78(9) 1_465 . ? 
O9 Ba1 O3 69.69(10) 1_455 . ? 
O12 Ba1 O3 67.25(10) . . ? 
O10 Ba1 O3 108.84(9) 1_465 . ? 
O1 Ba1 O3 46.24(9) . . ? 
O9 Ba1 O4 165.02(7) 1_455 . ? 
O12 Ba1 O4 51.26(7) . . ? 
O10 Ba1 O4 70.94(8) 1_465 . ? 
O1 Ba1 O4 85.59(10) . . ? 
O3 Ba1 O4 96.68(9) . . ? 
O9 Ba1 O4 116.47(8) 1_455 2_665 ? 
O12 Ba1 O4 104.42(8) . 2_665 ? 
O10 Ba1 O4 73.85(9) 1_465 2_665 ? 
O1 Ba1 O4 136.45(8) . 2_665 ? 
O3 Ba1 O4 171.60(10) . 2_665 ? 
O4 Ba1 O4 76.50(8) . 2_665 ? 
O9 Ba1 O11 70.55(8) 1_455 1_465 ? 
O12 Ba1 O11 162.31(8) . 1_465 ? 
O10 Ba1 O11 48.96(8) 1_465 1_465 ? 
O1 Ba1 O11 69.08(9) . 1_465 ? 
O3 Ba1 O11 101.80(9) . 1_465 ? 
O4 Ba1 O11 119.91(7) . 1_465 ? 
O4 Ba1 O11 85.99(8) 2_665 1_465 ? 
O9 Ba1 O5 49.04(8) 1_455 1_545 ? 
O12 Ba1 O5 68.83(7) . 1_545 ? 
O10 Ba1 O5 165.63(9) 1_465 1_545 ? 
O1 Ba1 O5 106.63(9) . 1_545 ? 
O3 Ba1 O5 62.16(8) . 1_545 ? 
O4 Ba1 O5 119.67(7) . 1_545 ? 
O4 Ba1 O5 116.77(7) 2_665 1_545 ? 
O11 Ba1 O5 119.57(7) 1_465 1_545 ? 
O9 Ba1 O5 99.33(8) 1_455 2_665 ? 
O12 Ba1 O5 72.45(8) . 2_665 ? 
O10 Ba1 O5 121.18(8) 1_465 2_665 ? 
O1 Ba1 O5 166.08(9) . 2_665 ? 
O3 Ba1 O5 126.57(8) . 2_665 ? 
O4 Ba1 O5 83.63(8) . 2_665 ? 
O4 Ba1 O5 48.54(7) 2_665 2_665 ? 
O11 Ba1 O5 124.22(7) 1_465 2_665 ? 
O5 Ba1 O5 71.54(8) 1_545 2_665 ? 
O9 Ba1 O11 70.07(8) 1_455 2_655 ? 
O12 Ba1 O11 118.03(8) . 2_655 ? 
O10 Ba1 O11 104.31(8) 1_465 2_655 ? 
O1 Ba1 O11 146.81(10) . 2_655 ? 
O3 Ba1 O11 136.50(8) . 2_655 ? 
O4 Ba1 O11 120.62(7) . 2_655 ? 
O4 Ba1 O11 47.54(7) 2_665 2_655 ? 
O11 Ba1 O11 79.58(9) 1_465 2_655 ? 
O5 Ba1 O11 79.19(7) 1_545 2_655 ? 
O5 Ba1 O11 47.08(7) 2_665 2_655 ? 
O9 Ba1 B2 96.63(10) 1_455 2_665 ? 
O12 Ba1 B2 98.72(11) . 2_665 ? 
O10 Ba1 B2 100.10(10) 1_465 2_665 ? 
O1 Ba1 B2 162.39(10) . 2_665 ? 
O3 Ba1 B2 151.07(10) . 2_665 ? 
O4 Ba1 B2 92.74(10) . 2_665 ? 
O4 Ba1 B2 27.55(9) 2_665 2_665 ? 
O11 Ba1 B2 96.97(10) 1_465 2_665 ? 
O5 Ba1 B2 89.44(9) 1_545 2_665 ? 
O5 Ba1 B2 27.89(9) 2_665 2_665 ? 
O11 Ba1 B2 28.14(9) 2_655 2_665 ? 
OW1 Ba2 O15 82.78(12) . 1_455 ? 
OW1 Ba2 O21 86.46(14) . . ? 
O15 Ba2 O21 114.16(8) 1_455 . ? 
OW1 Ba2 O13 67.69(10) . 1_465 ? 
O15 Ba2 O13 117.53(8) 1_455 1_465 ? 
O21 Ba2 O13 117.18(8) . 1_465 ? 
OW1 Ba2 O20 144.28(10) . 2_676 ? 
O15 Ba2 O20 105.87(8) 1_455 2_676 ? 
O21 Ba2 O20 118.84(8) . 2_676 ? 
O13 Ba2 O20 77.90(8) 1_465 2_676 ? 
OW1 Ba2 O20 81.47(14) . 1_455 ? 
O15 Ba2 O20 51.45(8) 1_455 1_455 ? 
O21 Ba2 O20 162.19(8) . 1_455 ? 
O13 Ba2 O20 69.99(7) 1_465 1_455 ? 
O20 Ba2 O20 77.96(8) 2_676 1_455 ? 
OW1 Ba2 O14 74.42(11) . 1_465 ? 
O15 Ba2 O14 156.67(7) 1_455 1_465 ? 
O21 Ba2 O14 69.81(8) . 1_465 ? 
O13 Ba2 O14 48.78(8) 1_465 1_465 ? 
O20 Ba2 O14 90.35(8) 2_676 1_465 ? 
O20 Ba2 O14 118.72(7) 1_455 1_465 ? 
OW1 Ba2 O19 94.32(10) . 1_545 ? 
O15 Ba2 O19 67.98(8) 1_455 1_545 ? 
O21 Ba2 O19 48.38(7) . 1_545 ? 
O13 Ba2 O19 159.15(8) 1_465 1_545 ? 
O20 Ba2 O19 121.21(7) 2_676 1_545 ? 
O20 Ba2 O19 119.38(7) 1_455 1_545 ? 
O14 Ba2 O19 117.92(8) 1_465 1_545 ? 
OW1 Ba2 O14 153.26(13) . 2_766 ? 
O15 Ba2 O14 119.76(7) 1_455 2_766 ? 
O21 Ba2 O14 71.63(8) . 2_766 ? 
O13 Ba2 O14 108.45(8) 1_465 2_766 ? 
O20 Ba2 O14 48.39(7) 2_676 2_766 ? 
O20 Ba2 O14 123.16(8) 1_455 2_766 ? 
O14 Ba2 O14 83.54(7) 1_465 2_766 ? 
O19 Ba2 O14 82.65(7) 1_545 2_766 ? 
OW1 Ba2 O19 157.26(11) . 2_676 ? 
O15 Ba2 O19 74.60(8) 1_455 2_676 ? 
O21 Ba2 O19 100.57(8) . 2_676 ? 
O13 Ba2 O19 125.30(8) 1_465 2_676 ? 
O20 Ba2 O19 48.66(7) 2_676 2_676 ? 
O20 Ba2 O19 86.15(7) 1_455 2_676 ? 
O14 Ba2 O19 128.33(7) 1_465 2_676 ? 
O19 Ba2 O19 75.26(9) 1_545 2_676 ? 
O14 Ba2 O19 46.87(7) 2_766 2_676 ? 
OW1 Ba2 B11 172.03(11) . 2_676 ? 
O15 Ba2 B11 100.72(10) 1_455 2_676 ? 
O21 Ba2 B11 98.48(10) . 2_676 ? 
O13 Ba2 B11 104.40(10) 1_465 2_676 ? 
O20 Ba2 B11 27.88(9) 2_676 2_676 ? 
O20 Ba2 B11 95.05(10) 1_455 2_676 ? 
O14 Ba2 B11 101.32(9) 1_465 2_676 ? 
O19 Ba2 B11 93.64(9) 1_545 2_676 ? 
O14 Ba2 B11 28.36(9) 2_766 2_676 ? 
O19 Ba2 B11 27.79(9) 2_676 2_676 ? 
OW1 Ba2 B7 90.37(13) . . ? 
O15 Ba2 B7 91.41(10) 1_455 . ? 
O21 Ba2 B7 23.85(9) . . ? 
O13 Ba2 B7 139.38(10) 1_465 . ? 
O20 Ba2 B7 123.24(9) 2_676 . ? 
O20 Ba2 B7 142.58(9) 1_455 . ? 
O14 Ba2 B7 93.53(9) 1_465 . ? 
O19 Ba2 B7 24.53(9) 1_545 . ? 
O14 Ba2 B7 75.86(9) 2_766 . ? 
O19 Ba2 B7 87.95(9) 2_676 . ? 
B11 Ba2 B7 96.67(11) 2_676 . ? 
O1 B1 O2 125.0(5) . . ? 
O1 B1 O3 111.9(4) . . ? 
O2 B1 O3 123.1(4) . . ? 
O1 B1 Ba1 55.6(3) . . ? 
O2 B1 Ba1 176.6(4) . . ? 
O3 B1 Ba1 56.4(2) . . ? 
O6 B2 O4 112.0(3) . . ? 
O6 B2 O5 111.3(3) . . ? 
O4 B2 O5 109.7(3) . . ? 
O6 B2 O11 110.6(3) . 1_565 ? 
O4 B2 O11 106.9(3) . 1_565 ? 
O5 B2 O11 106.1(3) . 1_565 ? 
O6 B2 Ba1 178.2(3) . 2_665 ? 
O4 B2 Ba1 66.3(2) . 2_665 ? 
O5 B2 Ba1 69.1(2) . 2_665 ? 
O11 B2 Ba1 70.8(2) 1_565 2_665 ? 
O8 B3 O7 120.8(3) . . ? 
O8 B3 O6 122.5(4) . . ? 
O7 B3 O6 116.7(4) . . ? 
O4 B4 O8 111.5(3) . . ? 
O4 B4 O9 111.9(3) . . ? 
O8 B4 O9 109.1(3) . . ? 
O4 B4 O12 109.0(3) . . ? 
O8 B4 O12 107.8(3) . . ? 
O9 B4 O12 107.4(3) . . ? 
O4 B4 Ba1 61.42(18) . . ? 
O8 B4 Ba1 106.1(3) . . ? 
O9 B4 Ba1 143.7(3) . . ? 
O12 B4 Ba1 52.09(17) . . ? 
O9 B5 O5 118.7(3) . 1_645 ? 
O9 B5 O10 119.0(4) . . ? 
O5 B5 O10 122.2(4) 1_645 . ? 
O9 B5 Ba1 52.23(19) . 1_655 ? 
O5 B5 Ba1 66.47(19) 1_645 1_655 ? 
O10 B5 Ba1 170.7(3) . 1_655 ? 
O12 B6 O11 127.2(4) . . ? 
O12 B6 O10 118.2(3) . . ? 
O11 B6 O10 114.5(3) . . ? 
O12 B6 Ba1 169.7(3) . 1_645 ? 
O11 B6 Ba1 62.9(2) . 1_645 ? 
O10 B6 Ba1 51.62(18) . 1_645 ? 
O19 B7 O21 117.1(4) 1_545 . ? 
O19 B7 O13 123.0(3) 1_545 . ? 
O21 B7 O13 119.6(4) . . ? 
O19 B7 Ba2 65.3(2) 1_545 . ? 
O21 B7 Ba2 51.8(2) . . ? 
O13 B7 Ba2 170.3(3) . . ? 
O15 B8 O14 126.9(4) . . ? 
O15 B8 O13 118.1(4) . . ? 
O14 B8 O13 114.8(3) . . ? 
O15 B8 Ba2 168.2(3) . 1_645 ? 
O14 B8 Ba2 62.85(19) . 1_645 ? 
O13 B8 Ba2 52.06(17) . 1_645 ? 
O20 B9 O16 112.9(3) . . ? 
O20 B9 O21 111.2(4) . . ? 
O16 B9 O21 108.7(3) . . ? 
O20 B9 O15 109.3(3) . . ? 
O16 B9 O15 107.7(3) . . ? 
O21 B9 O15 106.8(3) . . ? 
O20 B9 Ba2 60.78(18) . 1_655 ? 
O16 B9 Ba2 110.5(3) . 1_655 ? 
O21 B9 Ba2 139.6(2) . 1_655 ? 
O15 B9 Ba2 51.68(16) . 1_655 ? 
O17 B10 O18 122.2(3) . . ? 
O17 B10 O16 115.6(4) . . ? 
O18 B10 O16 122.2(4) . . ? 
O18 B11 O20 112.8(3) . . ? 
O18 B11 O19 111.1(3) . . ? 
O20 B11 O19 109.5(3) . . ? 
O18 B11 O14 111.1(3) . 1_465 ? 
O20 B11 O14 106.5(3) . 1_465 ? 
O19 B11 O14 105.5(3) . 1_465 ? 
O18 B11 Ba2 177.0(3) . 2_676 ? 
O20 B11 Ba2 64.32(19) . 2_676 ? 
O19 B11 Ba2 71.0(2) . 2_676 ? 
O14 B11 Ba2 69.78(19) 1_465 2_676 ? 
Ba2 OW1 HW1 127(4) . . ? 
Ba2 OW1 HW2 124(4) . . ? 
HW1 OW1 HW2 108.3(18) . . ? 
B1 O1 Ba1 101.3(3) . . ? 
B1 O1 H1 117(4) . . ? 
Ba1 O1 H1 139(4) . . ? 
B1 O2 H2 118(4) . . ? 
B1 O3 Ba1 100.4(2) . . ? 
B1 O3 H3 121(4) . . ? 
Ba1 O3 H3 138(4) . . ? 
B4 O4 B2 119.8(3) . . ? 
B4 O4 Ba1 92.3(2) . . ? 
B2 O4 Ba1 124.4(2) . . ? 
B4 O4 Ba1 133.7(3) . 2_665 ? 
B2 O4 Ba1 86.2(2) . 2_665 ? 
Ba1 O4 Ba1 103.50(8) . 2_665 ? 
B5 O5 B2 130.3(3) 1_465 . ? 
B5 O5 Ba1 88.6(2) 1_465 1_565 ? 
B2 O5 Ba1 127.7(2) . 1_565 ? 
B5 O5 Ba1 120.1(2) 1_465 2_665 ? 
B2 O5 Ba1 83.0(2) . 2_665 ? 
Ba1 O5 Ba1 108.46(8) 1_565 2_665 ? 
B3 O6 B2 120.1(3) . . ? 
B3 O7 H7 117(4) . . ? 
B3 O8 B4 122.1(3) . . ? 
B5 O9 B4 123.0(3) . . ? 
B5 O9 Ba1 103.6(2) . 1_655 ? 
B4 O9 Ba1 131.2(2) . 1_655 ? 
B5 O10 B6 121.2(3) . . ? 
B5 O10 Ba1 134.2(3) . 1_645 ? 
B6 O10 Ba1 103.7(2) . 1_645 ? 
B6 O11 B2 132.0(3) . 1_545 ? 
B6 O11 Ba1 92.8(2) . 1_645 ? 
B2 O11 Ba1 128.1(2) 1_545 1_645 ? 
B6 O11 Ba1 119.3(2) . 2_655 ? 
B2 O11 Ba1 81.1(2) 1_545 2_655 ? 
Ba1 O11 Ba1 100.42(9) 1_645 2_655 ? 
B6 O12 B4 124.0(3) . . ? 
B6 O12 Ba1 134.0(3) . . ? 
B4 O12 Ba1 101.4(2) . . ? 
B7 O13 B8 121.1(3) . . ? 
B7 O13 Ba2 133.2(2) . 1_645 ? 
B8 O13 Ba2 103.3(2) . 1_645 ? 
B8 O14 B11 132.5(3) . 1_645 ? 
B8 O14 Ba2 92.9(2) . 1_645 ? 
B11 O14 Ba2 129.2(2) 1_645 1_645 ? 
B8 O14 Ba2 118.6(2) . 2_766 ? 
B11 O14 Ba2 81.86(19) 1_645 2_766 ? 
Ba2 O14 Ba2 96.46(7) 1_645 2_766 ? 
B8 O15 B9 123.5(3) . . ? 
B8 O15 Ba2 134.0(2) . 1_655 ? 
B9 O15 Ba2 101.7(2) . 1_655 ? 
B10 O16 B9 122.2(3) . . ? 
B10 O17 H17 107(4) . . ? 
B10 O18 B11 119.5(3) . . ? 
B7 O19 B11 130.9(3) 1_565 . ? 
B7 O19 Ba2 90.2(2) 1_565 1_565 ? 
B11 O19 Ba2 130.6(2) . 1_565 ? 
B7 O19 Ba2 118.1(2) 1_565 2_676 ? 
B11 O19 Ba2 81.2(2) . 2_676 ? 
Ba2 O19 Ba2 104.74(9) 1_565 2_676 ? 
B9 O20 B11 118.5(3) . . ? 
B9 O20 Ba2 132.1(2) . 2_676 ? 
B11 O20 Ba2 87.8(2) . 2_676 ? 
B9 O20 Ba2 93.3(2) . 1_655 ? 
B11 O20 Ba2 126.2(2) . 1_655 ? 
Ba2 O20 Ba2 102.04(8) 2_676 1_655 ? 
B7 O21 B9 120.5(3) . . ? 
B7 O21 Ba2 104.4(2) . . ? 
B9 O21 Ba2 131.3(2) . . ? 
 
loop_ 
 _geom_torsion_atom_site_label_1 
 _geom_torsion_atom_site_label_2 
 _geom_torsion_atom_site_label_3 
 _geom_torsion_atom_site_label_4 
 _geom_torsion 
 _geom_torsion_site_symmetry_1 
 _geom_torsion_site_symmetry_2 
 _geom_torsion_site_symmetry_3 
 _geom_torsion_site_symmetry_4 
 _geom_torsion_publ_flag 
O9 Ba1 B1 O1 -113.3(3) 1_455 . . . ? 
O12 Ba1 B1 O1 128.0(3) . . . . ? 
O10 Ba1 B1 O1 6.8(3) 1_465 . . . ? 
O3 Ba1 B1 O1 -176.2(5) . . . . ? 
O4 Ba1 B1 O1 77.7(3) . . . . ? 
O4 Ba1 B1 O1 25.5(5) 2_665 . . . ? 
O11 Ba1 B1 O1 -42.3(3) 1_465 . . . ? 
O5 Ba1 B1 O1 -162.6(3) 1_545 . . . ? 
O5 Ba1 B1 O1 156.2(2) 2_665 . . . ? 
O11 Ba1 B1 O1 -103.9(3) 2_655 . . . ? 
B2 Ba1 B1 O1 -159.8(11) 2_665 . . . ? 
O9 Ba1 B1 O2 145(5) 1_455 . . . ? 
O12 Ba1 B1 O2 26(5) . . . . ? 
O10 Ba1 B1 O2 -95(5) 1_465 . . . ? 
O1 Ba1 B1 O2 -102(5) . . . . ? 
O3 Ba1 B1 O2 82(5) . . . . ? 
O4 Ba1 B1 O2 -24(5) . . . . ? 
O4 Ba1 B1 O2 -77(5) 2_665 . . . ? 
O11 Ba1 B1 O2 -144(5) 1_465 . . . ? 
O5 Ba1 B1 O2 95(5) 1_545 . . . ? 
O5 Ba1 B1 O2 54(5) 2_665 . . . ? 
O11 Ba1 B1 O2 154(5) 2_655 . . . ? 
B2 Ba1 B1 O2 98(5) 2_665 . . . ? 
O9 Ba1 B1 O3 62.9(3) 1_455 . . . ? 
O12 Ba1 B1 O3 -55.8(3) . . . . ? 
O10 Ba1 B1 O3 -177.0(3) 1_465 . . . ? 
O1 Ba1 B1 O3 176.2(5) . . . . ? 
O4 Ba1 B1 O3 -106.1(3) . . . . ? 
O4 Ba1 B1 O3 -158.3(3) 2_665 . . . ? 
O11 Ba1 B1 O3 133.9(3) 1_465 . . . ? 
O5 Ba1 B1 O3 13.7(3) 1_545 . . . ? 
O5 Ba1 B1 O3 -27.5(4) 2_665 . . . ? 
O11 Ba1 B1 O3 72.3(4) 2_655 . . . ? 
B2 Ba1 B1 O3 16.4(14) 2_665 . . . ? 
O9 Ba1 B4 O4 -174.12(18) 1_455 . . . ? 
O12 Ba1 B4 O4 153.5(4) . . . . ? 
O10 Ba1 B4 O4 -31.5(2) 1_465 . . . ? 
O1 Ba1 B4 O4 -93.6(2) . . . . ? 
O3 Ba1 B4 O4 -140.1(2) . . . . ? 
O4 Ba1 B4 O4 42.6(3) 2_665 . . . ? 
O11 Ba1 B4 O4 -48.1(3) 1_465 . . . ? 
O5 Ba1 B4 O4 160.2(2) 1_545 . . . ? 
O5 Ba1 B4 O4 89.5(2) 2_665 . . . ? 
O11 Ba1 B4 O4 80.0(2) 2_655 . . . ? 
B2 Ba1 B4 O4 69.6(2) 2_665 . . . ? 
O9 Ba1 B4 O8 -68.0(3) 1_455 . . . ? 
O12 Ba1 B4 O8 -100.3(3) . . . . ? 
O10 Ba1 B4 O8 74.6(2) 1_465 . . . ? 
O1 Ba1 B4 O8 12.5(2) . . . . ? 
O3 Ba1 B4 O8 -34.0(2) . . . . ? 
O4 Ba1 B4 O8 106.1(3) . . . . ? 
O4 Ba1 B4 O8 148.7(2) 2_665 . . . ? 
O11 Ba1 B4 O8 58.0(3) 1_465 . . . ? 
O5 Ba1 B4 O8 -93.7(2) 1_545 . . . ? 
O5 Ba1 B4 O8 -164.3(2) 2_665 . . . ? 
O11 Ba1 B4 O8 -173.93(17) 2_655 . . . ? 
B2 Ba1 B4 O8 175.7(2) 2_665 . . . ? 
O9 Ba1 B4 O9 97.4(4) 1_455 . . . ? 
O12 Ba1 B4 O9 65.0(4) . . . . ? 
O10 Ba1 B4 O9 -120.0(4) 1_465 . . . ? 
O1 Ba1 B4 O9 177.9(4) . . . . ? 
O3 Ba1 B4 O9 131.4(4) . . . . ? 
O4 Ba1 B4 O9 -88.5(4) . . . . ? 
O4 Ba1 B4 O9 -45.9(4) 2_665 . . . ? 
O11 Ba1 B4 O9 -136.6(3) 1_465 . . . ? 
O5 Ba1 B4 O9 71.7(4) 1_545 . . . ? 
O5 Ba1 B4 O9 1.0(4) 2_665 . . . ? 
O11 Ba1 B4 O9 -8.6(4) 2_655 . . . ? 
B2 Ba1 B4 O9 -18.9(4) 2_665 . . . ? 
O9 Ba1 B4 O12 32.3(3) 1_455 . . . ? 
O10 Ba1 B4 O12 175.0(2) 1_465 . . . ? 
O1 Ba1 B4 O12 112.8(2) . . . . ? 
O3 Ba1 B4 O12 66.3(2) . . . . ? 
O4 Ba1 B4 O12 -153.5(4) . . . . ? 
O4 Ba1 B4 O12 -111.0(2) 2_665 . . . ? 
O11 Ba1 B4 O12 158.38(18) 1_465 . . . ? 
O5 Ba1 B4 O12 6.7(2) 1_545 . . . ? 
O5 Ba1 B4 O12 -64.0(2) 2_665 . . . ? 
O11 Ba1 B4 O12 -73.6(2) 2_655 . . . ? 
B2 Ba1 B4 O12 -83.9(2) 2_665 . . . ? 
OW1 Ba2 B7 O19 -99.6(2) . . . 1_545 ? 
O15 Ba2 B7 O19 -16.8(2) 1_455 . . 1_545 ? 
O21 Ba2 B7 O19 -180.0(4) . . . 1_545 ? 
O13 Ba2 B7 O19 -154.48(18) 1_465 . . 1_545 ? 
O20 Ba2 B7 O19 93.2(2) 2_676 . . 1_545 ? 
O20 Ba2 B7 O19 -23.3(3) 1_455 . . 1_545 ? 
O14 Ba2 B7 O19 -174.0(2) 1_465 . . 1_545 ? 
O14 Ba2 B7 O19 103.5(2) 2_766 . . 1_545 ? 
O19 Ba2 B7 O19 57.7(2) 2_676 . . 1_545 ? 
B11 Ba2 B7 O19 84.1(2) 2_676 . . 1_545 ? 
OW1 Ba2 B7 O21 80.4(3) . . . . ? 
O15 Ba2 B7 O21 163.1(2) 1_455 . . . ? 
O13 Ba2 B7 O21 25.5(3) 1_465 . . . ? 
O20 Ba2 B7 O21 -86.8(2) 2_676 . . . ? 
O20 Ba2 B7 O21 156.7(2) 1_455 . . . ? 
O14 Ba2 B7 O21 5.9(2) 1_465 . . . ? 
O19 Ba2 B7 O21 180.0(4) 1_545 . . . ? 
O14 Ba2 B7 O21 -76.5(2) 2_766 . . . ? 
O19 Ba2 B7 O21 -122.3(2) 2_676 . . . ? 
B11 Ba2 B7 O21 -95.9(2) 2_676 . . . ? 
OW1 Ba2 B7 O13 109.6(17) . . . . ? 
O15 Ba2 B7 O13 -167.6(17) 1_455 . . . ? 
O21 Ba2 B7 O13 29.2(16) . . . . ? 
O13 Ba2 B7 O13 54.7(17) 1_465 . . . ? 
O20 Ba2 B7 O13 -57.6(17) 2_676 . . . ? 
O20 Ba2 B7 O13 -174.1(16) 1_455 . . . ? 
O14 Ba2 B7 O13 35.2(17) 1_465 . . . ? 
O19 Ba2 B7 O13 -150.8(18) 1_545 . . . ? 
O14 Ba2 B7 O13 -47.3(17) 2_766 . . . ? 
O19 Ba2 B7 O13 -93.1(17) 2_676 . . . ? 
B11 Ba2 B7 O13 -66.7(17) 2_676 . . . ? 
O2 B1 O1 Ba1 175.9(5) . . . . ? 
O3 B1 O1 Ba1 -3.4(5) . . . . ? 
O9 Ba1 O1 B1 64.5(3) 1_455 . . . ? 
O12 Ba1 O1 B1 -50.9(3) . . . . ? 
O10 Ba1 O1 B1 -172.4(3) 1_465 . . . ? 
O3 Ba1 O1 B1 2.1(3) . . . . ? 
O4 Ba1 O1 B1 -101.5(3) . . . . ? 
O4 Ba1 O1 B1 -166.7(3) 2_665 . . . ? 
O11 Ba1 O1 B1 134.1(3) 1_465 . . . ? 
O5 Ba1 O1 B1 18.1(3) 1_545 . . . ? 
O5 Ba1 O1 B1 -62.2(5) 2_665 . . . ? 
O11 Ba1 O1 B1 113.8(3) 2_655 . . . ? 
B2 Ba1 O1 B1 173.3(4) 2_665 . . . ? 
O1 B1 O3 Ba1 3.4(5) . . . . ? 
O2 B1 O3 Ba1 -175.9(5) . . . . ? 
O9 Ba1 O3 B1 -111.1(3) 1_455 . . . ? 
O12 Ba1 O3 B1 118.2(3) . . . . ? 
O10 Ba1 O3 B1 3.2(3) 1_465 . . . ? 
O1 Ba1 O3 B1 -2.0(3) . . . . ? 
O4 Ba1 O3 B1 75.3(3) . . . . ? 
O4 Ba1 O3 B1 110.6(6) 2_665 . . . ? 
O11 Ba1 O3 B1 -47.2(3) 1_465 . . . ? 
O5 Ba1 O3 B1 -164.6(3) 1_545 . . . ? 
O5 Ba1 O3 B1 162.3(3) 2_665 . . . ? 
O11 Ba1 O3 B1 -134.4(3) 2_655 . . . ? 
B2 Ba1 O3 B1 -176.6(3) 2_665 . . . ? 
O8 B4 O4 B2 35.4(5) . . . . ? 
O9 B4 O4 B2 -87.1(4) . . . . ? 
O12 B4 O4 B2 154.4(4) . . . . ? 
Ba1 B4 O4 B2 132.5(3) . . . . ? 
O8 B4 O4 Ba1 -97.1(3) . . . . ? 
O9 B4 O4 Ba1 140.4(3) . . . . ? 
O12 B4 O4 Ba1 21.8(3) . . . . ? 
O8 B4 O4 Ba1 151.6(2) . . . 2_665 ? 
O9 B4 O4 Ba1 29.1(5) . . . 2_665 ? 
O12 B4 O4 Ba1 -89.4(4) . . . 2_665 ? 
Ba1 B4 O4 Ba1 -111.3(3) . . . 2_665 ? 
O6 B2 O4 B4 -41.3(5) . . . . ? 
O5 B2 O4 B4 -165.3(3) . . . . ? 
O11 B2 O4 B4 80.1(4) 1_565 . . . ? 
Ba1 B2 O4 B4 139.5(3) 2_665 . . . ? 
O6 B2 O4 Ba1 75.5(4) . . . . ? 
O5 B2 O4 Ba1 -48.6(4) . . . . ? 
O11 B2 O4 Ba1 -163.15(18) 1_565 . . . ? 
Ba1 B2 O4 Ba1 -103.74(18) 2_665 . . . ? 
O6 B2 O4 Ba1 179.3(3) . . . 2_665 ? 
O5 B2 O4 Ba1 55.2(3) . . . 2_665 ? 
O11 B2 O4 Ba1 -59.4(2) 1_565 . . 2_665 ? 
O9 Ba1 O4 B4 15.0(4) 1_455 . . . ? 
O12 Ba1 O4 B4 -14.8(2) . . . . ? 
O10 Ba1 O4 B4 146.5(2) 1_465 . . . ? 
O1 Ba1 O4 B4 83.8(2) . . . . ? 
O3 Ba1 O4 B4 38.8(2) . . . . ? 
O4 Ba1 O4 B4 -136.2(3) 2_665 . . . ? 
O11 Ba1 O4 B4 146.6(2) 1_465 . . . ? 
O5 Ba1 O4 B4 -22.8(3) 1_545 . . . ? 
O5 Ba1 O4 B4 -87.4(2) 2_665 . . . ? 
O11 Ba1 O4 B4 -117.8(2) 2_655 . . . ? 
B2 Ba1 O4 B4 -113.8(2) 2_665 . . . ? 
O9 Ba1 O4 B2 -114.2(4) 1_455 . . . ? 
O12 Ba1 O4 B2 -144.0(3) . . . . ? 
O10 Ba1 O4 B2 17.3(3) 1_465 . . . ? 
O1 Ba1 O4 B2 -45.4(3) . . . . ? 
O3 Ba1 O4 B2 -90.3(3) . . . . ? 
O4 Ba1 O4 B2 94.6(3) 2_665 . . . ? 
O11 Ba1 O4 B2 17.4(3) 1_465 . . . ? 
O5 Ba1 O4 B2 -152.0(3) 1_545 . . . ? 
O5 Ba1 O4 B2 143.5(3) 2_665 . . . ? 
O11 Ba1 O4 B2 113.0(3) 2_655 . . . ? 
B2 Ba1 O4 B2 117.1(2) 2_665 . . . ? 
O9 Ba1 O4 Ba1 151.2(3) 1_455 . . 2_665 ? 
O12 Ba1 O4 Ba1 121.40(13) . . . 2_665 ? 
O10 Ba1 O4 Ba1 -77.31(9) 1_465 . . 2_665 ? 
O1 Ba1 O4 Ba1 -140.01(10) . . . 2_665 ? 
O3 Ba1 O4 Ba1 175.02(9) . . . 2_665 ? 
O4 Ba1 O4 Ba1 0.0 2_665 . . 2_665 ? 
O11 Ba1 O4 Ba1 -77.23(11) 1_465 . . 2_665 ? 
O5 Ba1 O4 Ba1 113.34(8) 1_545 . . 2_665 ? 
O5 Ba1 O4 Ba1 48.83(8) 2_665 . . 2_665 ? 
O11 Ba1 O4 Ba1 18.39(11) 2_655 . . 2_665 ? 
B2 Ba1 O4 Ba1 22.42(10) 2_665 . . 2_665 ? 
O6 B2 O5 B5 -54.1(5) . . . 1_465 ? 
O4 B2 O5 B5 70.4(5) . . . 1_465 ? 
O11 B2 O5 B5 -174.4(4) 1_565 . . 1_465 ? 
Ba1 B2 O5 B5 124.0(4) 2_665 . . 1_465 ? 
O6 B2 O5 Ba1 74.0(4) . . . 1_565 ? 
O4 B2 O5 Ba1 -161.5(2) . . . 1_565 ? 
O11 B2 O5 Ba1 -46.4(4) 1_565 . . 1_565 ? 
Ba1 B2 O5 Ba1 -108.0(2) 2_665 . . 1_565 ? 
O6 B2 O5 Ba1 -178.1(3) . . . 2_665 ? 
O4 B2 O5 Ba1 -53.6(3) . . . 2_665 ? 
O11 B2 O5 Ba1 61.6(3) 1_565 . . 2_665 ? 
O8 B3 O6 B2 -3.3(6) . . . . ? 
O7 B3 O6 B2 177.1(4) . . . . ? 
O4 B2 O6 B3 23.8(5) . . . . ? 
O5 B2 O6 B3 147.0(4) . . . . ? 
O11 B2 O6 B3 -95.4(4) 1_565 . . . ? 
Ba1 B2 O6 B3 46(9) 2_665 . . . ? 
O7 B3 O8 B4 176.7(4) . . . . ? 
O6 B3 O8 B4 -2.9(7) . . . . ? 
O4 B4 O8 B3 -12.6(5) . . . . ? 
O9 B4 O8 B3 111.5(4) . . . . ? 
O12 B4 O8 B3 -132.3(4) . . . . ? 
Ba1 B4 O8 B3 -77.6(4) . . . . ? 
O5 B5 O9 B4 -165.7(4) 1_645 . . . ? 
O10 B5 O9 B4 18.5(6) . . . . ? 
Ba1 B5 O9 B4 -165.0(4) 1_655 . . . ? 
O5 B5 O9 Ba1 -0.7(4) 1_645 . . 1_655 ? 
O10 B5 O9 Ba1 -176.5(3) . . . 1_655 ? 
O4 B4 O9 B5 -150.3(3) . . . . ? 
O8 B4 O9 B5 85.9(4) . . . . ? 
O12 B4 O9 B5 -30.7(5) . . . . ? 
Ba1 B4 O9 B5 -79.2(5) . . . . ? 
O4 B4 O9 Ba1 49.3(5) . . . 1_655 ? 
O8 B4 O9 Ba1 -74.5(4) . . . 1_655 ? 
O12 B4 O9 Ba1 168.87(19) . . . 1_655 ? 
Ba1 B4 O9 Ba1 120.3(3) . . . 1_655 ? 
O9 B5 O10 B6 2.8(6) . . . . ? 
O5 B5 O10 B6 -172.9(4) 1_645 . . . ? 
Ba1 B5 O10 B6 -15(2) 1_655 . . . ? 
O9 B5 O10 Ba1 170.1(2) . . . 1_645 ? 
O5 B5 O10 Ba1 -5.6(6) 1_645 . . 1_645 ? 
Ba1 B5 O10 Ba1 152.7(18) 1_655 . . 1_645 ? 
O12 B6 O10 B5 -7.2(6) . . . . ? 
O11 B6 O10 B5 169.1(4) . . . . ? 
Ba1 B6 O10 B5 170.7(4) 1_645 . . . ? 
O12 B6 O10 Ba1 -177.9(3) . . . 1_645 ? 
O11 B6 O10 Ba1 -1.6(4) . . . 1_645 ? 
O12 B6 O11 B2 -31.7(6) . . . 1_545 ? 
O10 B6 O11 B2 152.4(4) . . . 1_545 ? 
Ba1 B6 O11 B2 151.0(4) 1_645 . . 1_545 ? 
O12 B6 O11 Ba1 177.3(4) . . . 1_645 ? 
O10 B6 O11 Ba1 1.4(3) . . . 1_645 ? 
O12 B6 O11 Ba1 73.7(5) . . . 2_655 ? 
O10 B6 O11 Ba1 -102.2(3) . . . 2_655 ? 
Ba1 B6 O11 Ba1 -103.6(2) 1_645 . . 2_655 ? 
O11 B6 O12 B4 174.8(4) . . . . ? 
O10 B6 O12 B4 -9.4(6) . . . . ? 
Ba1 B6 O12 B4 -18.7(18) 1_645 . . . ? 
O11 B6 O12 Ba1 -16.2(6) . . . . ? 
O10 B6 O12 Ba1 159.6(2) . . . . ? 
Ba1 B6 O12 Ba1 150.3(14) 1_645 . . . ? 
O4 B4 O12 B6 147.5(4) . . . . ? 
O8 B4 O12 B6 -91.3(4) . . . . ? 
O9 B4 O12 B6 26.1(5) . . . . ? 
Ba1 B4 O12 B6 171.9(4) . . . . ? 
O4 B4 O12 Ba1 -24.4(4) . . . . ? 
O8 B4 O12 Ba1 96.8(3) . . . . ? 
O9 B4 O12 Ba1 -145.8(2) . . . . ? 
O9 Ba1 O12 B6 32.1(4) 1_455 . . . ? 
O10 Ba1 O12 B6 -176.5(3) 1_465 . . . ? 
O1 Ba1 O12 B6 122.8(4) . . . . ? 
O3 Ba1 O12 B6 84.1(4) . . . . ? 
O4 Ba1 O12 B6 -156.1(4) . . . . ? 
O4 Ba1 O12 B6 -97.1(4) 2_665 . . . ? 
O11 Ba1 O12 B6 138.3(3) 1_465 . . . ? 
O5 Ba1 O12 B6 16.4(3) 1_545 . . . ? 
O5 Ba1 O12 B6 -60.1(4) 2_665 . . . ? 
O11 Ba1 O12 B6 -47.8(4) 2_655 . . . ? 
B2 Ba1 O12 B6 -69.6(4) 2_665 . . . ? 
O9 Ba1 O12 B4 -157.2(2) 1_455 . . . ? 
O10 Ba1 O12 B4 -5.8(3) 1_465 . . . ? 
O1 Ba1 O12 B4 -66.5(2) . . . . ? 
O3 Ba1 O12 B4 -105.3(2) . . . . ? 
O4 Ba1 O12 B4 14.6(2) . . . . ? 
O4 Ba1 O12 B4 73.6(2) 2_665 . . . ? 
O11 Ba1 O12 B4 -51.1(4) 1_465 . . . ? 
O5 Ba1 O12 B4 -172.9(3) 1_545 . . . ? 
O5 Ba1 O12 B4 110.6(2) 2_665 . . . ? 
O11 Ba1 O12 B4 122.8(2) 2_655 . . . ? 
B2 Ba1 O12 B4 101.1(2) 2_665 . . . ? 
O19 B7 O13 B8 -174.6(4) 1_545 . . . ? 
O21 B7 O13 B8 -0.3(6) . . . . ? 
Ba2 B7 O13 B8 -26.5(19) . . . . ? 
O19 B7 O13 Ba2 -14.9(6) 1_545 . . 1_645 ? 
O21 B7 O13 Ba2 159.3(3) . . . 1_645 ? 
Ba2 B7 O13 Ba2 133.2(15) . . . 1_645 ? 
O15 B8 O13 B7 -7.2(6) . . . . ? 
O14 B8 O13 B7 169.0(4) . . . . ? 
Ba2 B8 O13 B7 164.9(4) 1_645 . . . ? 
O15 B8 O13 Ba2 -172.1(3) . . . 1_645 ? 
O14 B8 O13 Ba2 4.1(4) . . . 1_645 ? 
O15 B8 O14 B11 -33.0(7) . . . 1_645 ? 
O13 B8 O14 B11 151.1(4) . . . 1_645 ? 
Ba2 B8 O14 B11 154.7(4) 1_645 . . 1_645 ? 
O15 B8 O14 Ba2 172.2(4) . . . 1_645 ? 
O13 B8 O14 Ba2 -3.7(4) . . . 1_645 ? 
O15 B8 O14 Ba2 73.2(5) . . . 2_766 ? 
O13 B8 O14 Ba2 -102.6(3) . . . 2_766 ? 
Ba2 B8 O14 Ba2 -98.98(17) 1_645 . . 2_766 ? 
O14 B8 O15 B9 174.3(4) . . . . ? 
O13 B8 O15 B9 -9.9(6) . . . . ? 
Ba2 B8 O15 B9 -41.8(15) 1_645 . . . ? 
O14 B8 O15 Ba2 -18.3(7) . . . 1_655 ? 
O13 B8 O15 Ba2 157.4(2) . . . 1_655 ? 
Ba2 B8 O15 Ba2 125.6(12) 1_645 . . 1_655 ? 
O20 B9 O15 B8 150.2(4) . . . . ? 
O16 B9 O15 B8 -86.8(4) . . . . ? 
O21 B9 O15 B8 29.8(5) . . . . ? 
Ba2 B9 O15 B8 170.8(4) 1_655 . . . ? 
O20 B9 O15 Ba2 -20.5(3) . . . 1_655 ? 
O16 B9 O15 Ba2 102.5(3) . . . 1_655 ? 
O21 B9 O15 Ba2 -140.9(2) . . . 1_655 ? 
O17 B10 O16 B9 174.5(4) . . . . ? 
O18 B10 O16 B9 -6.0(7) . . . . ? 
O20 B9 O16 B10 -9.4(6) . . . . ? 
O21 B9 O16 B10 114.5(4) . . . . ? 
O15 B9 O16 B10 -130.2(4) . . . . ? 
Ba2 B9 O16 B10 -75.3(4) 1_655 . . . ? 
O17 B10 O18 B11 176.8(4) . . . . ? 
O16 B10 O18 B11 -2.6(7) . . . . ? 
O20 B11 O18 B10 25.0(5) . . . . ? 
O19 B11 O18 B10 148.3(4) . . . . ? 
O14 B11 O18 B10 -94.5(4) 1_465 . . . ? 
Ba2 B11 O18 B10 13(6) 2_676 . . . ? 
O18 B11 O19 B7 -58.1(5) . . . 1_565 ? 
O20 B11 O19 B7 67.2(5) . . . 1_565 ? 
O14 B11 O19 B7 -178.6(3) 1_465 . . 1_565 ? 
Ba2 B11 O19 B7 119.7(4) 2_676 . . 1_565 ? 
O18 B11 O19 Ba2 80.3(4) . . . 1_565 ? 
O20 B11 O19 Ba2 -154.5(2) . . . 1_565 ? 
O14 B11 O19 Ba2 -40.3(4) 1_465 . . 1_565 ? 
Ba2 B11 O19 Ba2 -101.9(2) 2_676 . . 1_565 ? 
O18 B11 O19 Ba2 -177.8(3) . . . 2_676 ? 
O20 B11 O19 Ba2 -52.6(3) . . . 2_676 ? 
O14 B11 O19 Ba2 61.6(2) 1_465 . . 2_676 ? 
O16 B9 O20 B11 33.3(5) . . . . ? 
O21 B9 O20 B11 -89.2(4) . . . . ? 
O15 B9 O20 B11 153.2(3) . . . . ? 
Ba2 B9 O20 B11 134.8(3) 1_655 . . . ? 
O16 B9 O20 Ba2 149.0(2) . . . 2_676 ? 
O21 B9 O20 Ba2 26.5(4) . . . 2_676 ? 
O15 B9 O20 Ba2 -91.2(4) . . . 2_676 ? 
Ba2 B9 O20 Ba2 -109.5(2) 1_655 . . 2_676 ? 
O16 B9 O20 Ba2 -101.5(3) . . . 1_655 ? 
O21 B9 O20 Ba2 136.0(3) . . . 1_655 ? 
O15 B9 O20 Ba2 18.4(3) . . . 1_655 ? 
O18 B11 O20 B9 -41.3(5) . . . . ? 
O19 B11 O20 B9 -165.6(3) . . . . ? 
O14 B11 O20 B9 80.8(4) 1_465 . . . ? 
Ba2 B11 O20 B9 138.0(3) 2_676 . . . ? 
O18 B11 O20 Ba2 -179.3(3) . . . 2_676 ? 
O19 B11 O20 Ba2 56.4(3) . . . 2_676 ? 
O14 B11 O20 Ba2 -57.2(3) 1_465 . . 2_676 ? 
O18 B11 O20 Ba2 77.3(4) . . . 1_655 ? 
O19 B11 O20 Ba2 -46.9(4) . . . 1_655 ? 
O14 B11 O20 Ba2 -160.50(19) 1_465 . . 1_655 ? 
Ba2 B11 O20 Ba2 -103.3(2) 2_676 . . 1_655 ? 
O19 B7 O21 B9 -160.4(3) 1_545 . . . ? 
O13 B7 O21 B9 25.0(5) . . . . ? 
Ba2 B7 O21 B9 -160.4(4) . . . . ? 
O19 B7 O21 Ba2 0.0(4) 1_545 . . . ? 
O13 B7 O21 Ba2 -174.6(3) . . . . ? 
O20 B9 O21 B7 -156.2(3) . . . . ? 
O16 B9 O21 B7 79.0(4) . . . . ? 
O15 B9 O21 B7 -37.0(5) . . . . ? 
Ba2 B9 O21 B7 -86.8(5) 1_655 . . . ? 
O20 B9 O21 Ba2 49.5(4) . . . . ? 
O16 B9 O21 Ba2 -75.4(4) . . . . ? 
O15 B9 O21 Ba2 168.6(2) . . . . ? 
Ba2 B9 O21 Ba2 118.8(3) 1_655 . . . ? 
OW1 Ba2 O21 B7 -99.0(3) . . . . ? 
O15 Ba2 O21 B7 -18.5(3) 1_455 . . . ? 
O13 Ba2 O21 B7 -161.6(2) 1_465 . . . ? 
O20 Ba2 O21 B7 107.6(2) 2_676 . . . ? 
O20 Ba2 O21 B7 -51.7(4) 1_455 . . . ? 
O14 Ba2 O21 B7 -173.7(3) 1_465 . . . ? 
O19 Ba2 O21 B7 0.0(2) 1_545 . . . ? 
O14 Ba2 O21 B7 96.6(2) 2_766 . . . ? 
O19 Ba2 O21 B7 59.2(2) 2_676 . . . ? 
B11 Ba2 O21 B7 87.3(2) 2_676 . . . ? 
OW1 Ba2 O21 B9 58.4(3) . . . . ? 
O15 Ba2 O21 B9 138.8(3) 1_455 . . . ? 
O13 Ba2 O21 B9 -4.3(3) 1_465 . . . ? 
O20 Ba2 O21 B9 -95.0(3) 2_676 . . . ? 
O20 Ba2 O21 B9 105.7(4) 1_455 . . . ? 
O14 Ba2 O21 B9 -16.3(3) 1_465 . . . ? 
O19 Ba2 O21 B9 157.4(4) 1_545 . . . ? 
O14 Ba2 O21 B9 -106.1(3) 2_766 . . . ? 
O19 Ba2 O21 B9 -143.4(3) 2_676 . . . ? 
B11 Ba2 O21 B9 -115.3(3) 2_676 . . . ? 
B7 Ba2 O21 B9 157.4(5) . . . . ? 
 
loop_ 
 _geom_hbond_atom_site_label_D 
 _geom_hbond_atom_site_label_H 
 _geom_hbond_atom_site_label_A 
 _geom_hbond_distance_DH 
 _geom_hbond_distance_HA 
 _geom_hbond_distance_DA 
 _geom_hbond_angle_DHA 
 _geom_hbond_site_symmetry_A 
OW1 HW2 O7  0.839(10) 1.860(17) 2.677(5) 164(5) . 
OW1 HW1 O2  0.837(10) 1.939(14) 2.770(5) 172(6) 1_565 
O2 H2 O16  0.856(10) 1.896(17) 2.742(5) 170(7) 1_455 
O3 H3 O6  0.852(10) 2.06(4) 2.738(4) 136(5) 1_545 
O7 H7 O18  0.848(10) 2.040(14) 2.883(4) 173(6) 1_545 
O17 H17 O8  0.844(10) 1.97(3) 2.755(4) 155(5) 1_565 
 
_diffrn_measured_fraction_theta_max    0.981 
_diffrn_reflns_theta_full              27.54 
_diffrn_measured_fraction_theta_full   0.981 
_refine_diff_density_max    1.453 
_refine_diff_density_min   -0.947 
_refine_diff_density_rms    0.214 

#===end

 
data_2 
 
_audit_creation_method            SHELXL-97 
_chemical_name_systematic 
; 
 ? 
; 
_chemical_name_common             ? 
_chemical_melting_point           ? 
_chemical_formula_moiety          ? 
_chemical_formula_sum 
 'B4 Ba Ga H3 O10' 
_chemical_formula_weight          413.32 
 
loop_ 
 _atom_type_symbol 
 _atom_type_description 
 _atom_type_scat_dispersion_real 
 _atom_type_scat_dispersion_imag 
 _atom_type_scat_source 
 'H'  'H'   0.0000   0.0000 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'B'  'B'   0.0013   0.0007 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'O'  'O'   0.0106   0.0060 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Ga'  'Ga'   0.2307   1.6083 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Ba'  'Ba'  -0.3244   2.2819 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 
_symmetry_cell_setting            triclinic 
_symmetry_space_group_name_H-M    P-1 
 
loop_ 
 _symmetry_equiv_pos_as_xyz 
 'x, y, z' 
 '-x, -y, -z' 
 
_cell_length_a                    7.1080(14) 
_cell_length_b                    7.1372(12) 
_cell_length_c                    9.878(3) 
_cell_angle_alpha                 106.885(17) 
_cell_angle_beta                  91.569(17) 
_cell_angle_gamma                 119.185(11) 
_cell_volume                      410.00(15) 
_cell_formula_units_Z             2 
_cell_measurement_temperature     296(2) 
_cell_measurement_reflns_used     2049 
_cell_measurement_theta_min       2.20 
_cell_measurement_theta_max       27.54 
 
_exptl_crystal_description        'lamellar' 
_exptl_crystal_colour             'colourless' 
_exptl_crystal_size_max           0.20 
_exptl_crystal_size_mid           0.14 
_exptl_crystal_size_min           0.03 
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_diffrn     3.348 
_exptl_crystal_density_method     'not measured' 
_exptl_crystal_F_000              380 
_exptl_absorpt_coefficient_mu     8.099 
_exptl_absorpt_correction_type    empirical 
_exptl_absorpt_correction_T_min   0.2942 
_exptl_absorpt_correction_T_max   0.7932 
_exptl_absorpt_process_details    'SADABS (Sheldrick, 1996)' 
 
_exptl_special_details 
; 
 ? 
; 
 
_diffrn_ambient_temperature       296(2) 
_diffrn_radiation_wavelength      0.71073 
_diffrn_radiation_type            MoK\a 
_diffrn_radiation_source          'fine-focus sealed tube' 
_diffrn_radiation_monochromator   graphite 
_diffrn_measurement_device_type   'Bruker APEX-II area-detector diffractometer' 
_diffrn_measurement_method        'phi and omega scans' 
_diffrn_detector_area_resol_mean  ? 
_diffrn_standards_number          none 
_diffrn_standards_interval_count  none 
_diffrn_standards_interval_time   none 
_diffrn_standards_decay_%         none 
_diffrn_reflns_number             5706 
_diffrn_reflns_av_R_equivalents   0.0517 
_diffrn_reflns_av_sigmaI/netI     0.0612 
_diffrn_reflns_limit_h_min        -9 
_diffrn_reflns_limit_h_max        9 
_diffrn_reflns_limit_k_min        -9 
_diffrn_reflns_limit_k_max        9 
_diffrn_reflns_limit_l_min        -12 
_diffrn_reflns_limit_l_max        12 
_diffrn_reflns_theta_min          2.20 
_diffrn_reflns_theta_max          27.54 
_reflns_number_total              1828 
_reflns_number_gt                 1505 
_reflns_threshold_expression      >2sigma(I) 
 
_computing_data_collection        'APEXII (Bruker, 2006)' 
_computing_cell_refinement        'SAINT (Bruker, 2006)' 
_computing_data_reduction         'SAINT' 
_computing_structure_solution     'SHELXS-97 (Sheldrick, 1990)' 
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)' 
_computing_molecular_graphics     'DIAMOND (Brandenburg, 1999)' 
_computing_publication_material   'SHELXTL (Sheldrick, 2008)' 
 
_refine_special_details 
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
; 
 
_refine_ls_structure_factor_coef  Fsqd  
_refine_ls_matrix_type            full 
_refine_ls_weighting_scheme       calc  
_refine_ls_weighting_details 
 'calc w=1/[σ²(Fo²)+(0.0388P)²+0.0000P] where P=(Fo²+2Fc²)/3' 
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap 
_atom_sites_solution_hydrogens    geom 
_refine_ls_hydrogen_treatment     mixed 
_refine_ls_extinction_method      none 
_refine_ls_extinction_coef        ? 
_refine_ls_number_reflns          1828 
_refine_ls_number_parameters      145 
_refine_ls_number_restraints      0 
_refine_ls_R_factor_all           0.0479 
_refine_ls_R_factor_gt            0.0324 
_refine_ls_wR_factor_ref          0.0866 
_refine_ls_wR_factor_gt           0.0651 
_refine_ls_goodness_of_fit_ref    1.154 
_refine_ls_restrained_S_all       1.154 
_refine_ls_shift/su_max           0.000 
_refine_ls_shift/su_mean          0.000 
 
loop_ 
 _atom_site_label 
 _atom_site_type_symbol 
 _atom_site_fract_x 
 _atom_site_fract_y 
 _atom_site_fract_z 
 _atom_site_U_iso_or_equiv 
 _atom_site_adp_type 
 _atom_site_occupancy 
 _atom_site_symmetry_multiplicity 
 _atom_site_calc_flag 
 _atom_site_refinement_flags 
 _atom_site_disorder_assembly 
 _atom_site_disorder_group 
Ba Ba 0.58052(7) 0.79322(6) 0.70709(4) 0.01440(14) Uani 1 1 d . . . 
Ga Ga 0.10876(12) 0.59013(11) 0.38242(7) 0.00956(18) Uani 1 1 d . . . 
B1 B 0.0602(14) 1.1355(12) 0.6563(8) 0.0121(16) Uani 1 1 d . . . 
B2 B 0.4386(13) 1.2496(11) 0.6448(8) 0.0094(14) Uani 1 1 d . . . 
B3 B 0.2040(13) 0.9026(11) 0.7078(8) 0.0094(15) Uani 1 1 d . . . 
B4 B 0.1271(14) 0.7390(13) 0.9094(9) 0.0153(17) Uani 1 1 d . . . 
O1 O 0.0333(8) 0.9593(7) 0.6989(5) 0.0132(10) Uani 1 1 d . . . 
OW1 O 0.6123(14) 0.6774(9) 0.9418(6) 0.052(2) Uani 1 1 d . . . 
H1A H 0.5217 0.6755 1.0040 0.078 Uiso 1 1 d R . . 
H1B H 0.7136 0.6408 0.9575 0.078 Uiso 1 1 d R . . 
O2 O -0.1196(8) 1.1455(7) 0.6212(5) 0.0131(10) Uani 1 1 d . . . 
O3 O 0.2685(8) 1.2975(7) 0.6449(5) 0.0130(10) Uani 1 1 d . . . 
O4 O 0.6168(8) 1.3876(7) 0.6009(5) 0.0134(10) Uani 1 1 d . . . 
O5 O 0.4110(8) 1.0684(7) 0.6793(5) 0.0122(10) Uani 1 1 d . . . 
O6 O 0.1327(8) 0.6750(7) 0.6024(4) 0.0096(9) Uani 1 1 d . . . 
O7 O 0.2569(8) 0.9085(7) 0.8542(5) 0.0151(11) Uani 1 1 d . . . 
O8 O -0.0399(10) 0.5326(8) 0.8283(5) 0.0227(12) Uani 1 1 d . . . 
O9 O 0.1870(10) 0.8037(8) 1.0576(5) 0.0246(13) Uani 1 1 d . . . 
H9A H 0.1342 0.6894 1.0806 0.037 Uiso 1 1 calc R . . 
 
 
_geom_special_details 
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
; 
 
loop_ 
 _geom_bond_atom_site_label_1 
 _geom_bond_atom_site_label_2 
 _geom_bond_distance 
 _geom_bond_site_symmetry_2 
 _geom_bond_publ_flag 
Ba OW1 2.717(6) . ? 
Ba O9 2.771(5) 2_677 ? 
Ba O2 2.774(4) 1_655 ? 
Ba O5 2.826(4) . ? 
Ba O1 2.850(5) 1_655 ? 
Ba O4 2.920(4) 1_545 ? 
Ba O6 2.934(5) . ? 
Ba O4 2.934(5) 2_676 ? 
Ba O3 2.970(4) 1_545 ? 
Ba O7 3.069(5) . ? 
Ba B3 3.131(8) . ? 
Ba B1 3.245(8) 1_655 ? 
Ga O2 1.862(4) 2_576 ? 
Ga O4 1.877(5) 2_676 ? 
Ga O6 1.887(4) 2_566 ? 
Ga O8 1.951(5) 2_566 ? 
Ga O6 2.057(4) . ? 
B1 O2 1.355(9) . ? 
B1 O1 1.369(8) . ? 
B1 O3 1.399(9) . ? 
B1 Ba 3.245(8) 1_455 ? 
B2 O4 1.351(9) . ? 
B2 O5 1.356(7) . ? 
B2 O3 1.408(8) . ? 
B2 Ba 3.349(6) 1_565 ? 
B2 Ba 3.393(7) 2_676 ? 
B3 O1 1.462(8) . ? 
B3 O7 1.468(8) . ? 
B3 O5 1.470(9) . ? 
B3 O6 1.471(8) . ? 
B4 O8 1.333(9) . ? 
B4 O9 1.386(9) . ? 
B4 O7 1.391(9) . ? 
O1 Ba 2.850(5) 1_455 ? 
OW1 H1A 0.8999 . ? 
OW1 H1B 0.9000 . ? 
O2 Ga 1.862(4) 2_576 ? 
O2 Ba 2.774(4) 1_455 ? 
O3 Ba 2.970(4) 1_565 ? 
O4 Ga 1.877(5) 2_676 ? 
O4 Ba 2.920(4) 1_565 ? 
O4 Ba 2.934(5) 2_676 ? 
O6 Ga 1.887(4) 2_566 ? 
O8 Ga 1.951(5) 2_566 ? 
O9 Ba 2.771(5) 2_677 ? 
O9 H9A 0.8200 . ? 
 
loop_ 
 _geom_angle_atom_site_label_1 
 _geom_angle_atom_site_label_2 
 _geom_angle_atom_site_label_3 
 _geom_angle 
 _geom_angle_site_symmetry_1 
 _geom_angle_site_symmetry_3 
 _geom_angle_publ_flag 
OW1 Ba O9 72.72(16) . 2_677 ? 
OW1 Ba O2 131.65(19) . 1_655 ? 
O9 Ba O2 69.59(14) 2_677 1_655 ? 
OW1 Ba O5 126.30(19) . . ? 
O9 Ba O5 74.28(15) 2_677 . ? 
O2 Ba O5 69.79(13) 1_655 . ? 
OW1 Ba O1 92.2(2) . 1_655 ? 
O9 Ba O1 74.31(16) 2_677 1_655 ? 
O2 Ba O1 49.23(12) 1_655 1_655 ? 
O5 Ba O1 117.78(13) . 1_655 ? 
OW1 Ba O4 74.42(17) . 1_545 ? 
O9 Ba O4 132.89(15) 2_677 1_545 ? 
O2 Ba O4 111.93(13) 1_655 1_545 ? 
O5 Ba O4 152.53(14) . 1_545 ? 
O1 Ba O4 74.20(13) 1_655 1_545 ? 
OW1 Ba O6 112.8(2) . . ? 
O9 Ba O6 113.66(15) 2_677 . ? 
O2 Ba O6 109.50(12) 1_655 . ? 
O5 Ba O6 48.64(12) . . ? 
O1 Ba O6 155.01(12) 1_655 . ? 
O4 Ba O6 109.73(13) 1_545 . ? 
OW1 Ba O4 144.41(15) . 2_676 ? 
O9 Ba O4 142.55(13) 2_677 2_676 ? 
O2 Ba O4 79.70(14) 1_655 2_676 ? 
O5 Ba O4 75.36(13) . 2_676 ? 
O1 Ba O4 101.60(14) 1_655 2_676 ? 
O4 Ba O4 78.03(13) 1_545 2_676 ? 
O6 Ba O4 57.05(13) . 2_676 ? 
OW1 Ba O3 69.13(16) . 1_545 ? 
O9 Ba O3 139.27(14) 2_677 1_545 ? 
O2 Ba O3 150.11(13) 1_655 1_545 ? 
O5 Ba O3 118.69(13) . 1_545 ? 
O1 Ba O3 120.29(12) 1_655 1_545 ? 
O4 Ba O3 46.47(13) 1_545 1_545 ? 
O6 Ba O3 70.24(12) . 1_545 ? 
O4 Ba O3 75.62(13) 2_676 1_545 ? 
OW1 Ba O7 82.5(2) . . ? 
O9 Ba O7 70.64(16) 2_677 . ? 
O2 Ba O7 111.36(12) 1_655 . ? 
O5 Ba O7 46.73(12) . . ? 
O1 Ba O7 144.54(13) 1_655 . ? 
O4 Ba O7 136.09(12) 1_545 . ? 
O6 Ba O7 47.16(12) . . ? 
O4 Ba O7 102.87(13) 2_676 . ? 
O3 Ba O7 90.57(12) 1_545 . ? 
OW1 Ba B3 108.9(2) . . ? 
O9 Ba B3 86.02(18) 2_677 . ? 
O2 Ba B3 97.64(16) 1_655 . ? 
O5 Ba B3 27.98(16) . . ? 
O1 Ba B3 145.55(15) 1_655 . ? 
O4 Ba B3 136.81(17) 1_545 . ? 
O6 Ba B3 27.83(15) . . ? 
O4 Ba B3 77.14(16) 2_676 . ? 
O3 Ba B3 93.09(16) 1_545 . ? 
O7 Ba B3 27.36(15) . . ? 
OW1 Ba B1 111.9(2) . 1_655 ? 
O9 Ba B1 68.34(18) 2_677 1_655 ? 
O2 Ba B1 24.45(15) 1_655 1_655 ? 
O5 Ba B1 93.20(16) . 1_655 ? 
O1 Ba B1 24.90(15) 1_655 1_655 ? 
O4 Ba B1 94.46(16) 1_545 1_655 ? 
O6 Ba B1 133.36(15) . 1_655 ? 
O4 Ba B1 92.14(16) 2_676 1_655 ? 
O3 Ba B1 140.40(15) 1_545 1_655 ? 
O7 Ba B1 129.02(15) . 1_655 ? 
B3 Ba B1 121.17(18) . 1_655 ? 
O2 Ga O4 114.4(2) 2_576 2_676 ? 
O2 Ga O6 128.0(2) 2_576 2_566 ? 
O4 Ga O6 117.00(19) 2_676 2_566 ? 
O2 Ga O8 90.0(2) 2_576 2_566 ? 
O4 Ga O8 94.9(2) 2_676 2_566 ? 
O6 Ga O8 93.1(2) 2_566 2_566 ? 
O2 Ga O6 94.35(18) 2_576 . ? 
O4 Ga O6 90.7(2) 2_676 . ? 
O6 Ga O6 77.79(19) 2_566 . ? 
O8 Ga O6 170.8(2) 2_566 . ? 
O2 B1 O1 118.7(7) . . ? 
O2 B1 O3 120.9(5) . . ? 
O1 B1 O3 120.4(6) . . ? 
O2 B1 Ba 57.9(3) . 1_455 ? 
O1 B1 Ba 61.2(4) . 1_455 ? 
O3 B1 Ba 175.1(5) . 1_455 ? 
O4 B2 O5 125.1(6) . . ? 
O4 B2 O3 114.8(5) . . ? 
O5 B2 O3 120.1(6) . . ? 
O4 B2 Ba 60.1(3) . 1_565 ? 
O5 B2 Ba 156.3(5) . 1_565 ? 
O3 B2 Ba 62.4(3) . 1_565 ? 
O4 B2 Ba 59.0(3) . 2_676 ? 
O5 B2 Ba 118.2(4) . 2_676 ? 
O3 B2 Ba 88.4(4) . 2_676 ? 
Ba B2 Ba 84.86(15) 1_565 2_676 ? 
O1 B3 O7 110.0(5) . . ? 
O1 B3 O5 112.2(5) . . ? 
O7 B3 O5 106.1(5) . . ? 
O1 B3 O6 110.9(6) . . ? 
O7 B3 O6 109.8(5) . . ? 
O5 B3 O6 107.6(5) . . ? 
O1 B3 Ba 175.7(4) . . ? 
O7 B3 Ba 73.9(3) . . ? 
O5 B3 Ba 64.4(3) . . ? 
O6 B3 Ba 68.6(3) . . ? 
O8 B4 O9 122.6(6) . . ? 
O8 B4 O7 123.6(7) . . ? 
O9 B4 O7 113.8(6) . . ? 
B1 O1 B3 123.0(6) . . ? 
B1 O1 Ba 93.9(4) . 1_455 ? 
B3 O1 Ba 142.6(4) . 1_455 ? 
Ba OW1 H1A 120.0 . . ? 
Ba OW1 H1B 120.0 . . ? 
H1A OW1 H1B 120.0 . . ? 
B1 O2 Ga 124.0(4) . 2_576 ? 
B1 O2 Ba 97.6(4) . 1_455 ? 
Ga O2 Ba 130.8(2) 2_576 1_455 ? 
B1 O3 B2 118.9(5) . . ? 
B1 O3 Ba 144.7(4) . 1_565 ? 
B2 O3 Ba 92.8(4) . 1_565 ? 
B2 O4 Ga 126.6(4) . 2_676 ? 
B2 O4 Ba 96.3(4) . 1_565 ? 
Ga O4 Ba 121.3(2) 2_676 1_565 ? 
B2 O4 Ba 97.8(4) . 2_676 ? 
Ga O4 Ba 108.36(19) 2_676 2_676 ? 
Ba O4 Ba 101.97(13) 1_565 2_676 ? 
B2 O5 B3 123.9(5) . . ? 
B2 O5 Ba 148.2(4) . . ? 
B3 O5 Ba 87.6(3) . . ? 
B3 O6 Ga 120.6(4) . 2_566 ? 
B3 O6 Ga 126.6(4) . . ? 
Ga O6 Ga 102.21(19) 2_566 . ? 
B3 O6 Ba 83.6(4) . . ? 
Ga O6 Ba 119.13(18) 2_566 . ? 
Ga O6 Ba 103.24(18) . . ? 
B4 O7 B3 124.8(6) . . ? 
B4 O7 Ba 108.9(4) . . ? 
B3 O7 Ba 78.7(3) . . ? 
B4 O8 Ga 125.4(5) . 2_566 ? 
B4 O9 Ba 137.7(4) . 2_677 ? 
B4 O9 H9A 109.5 . . ? 
Ba O9 H9A 112.8 2_677 . ? 
 
loop_ 
 _geom_torsion_atom_site_label_1 
 _geom_torsion_atom_site_label_2 
 _geom_torsion_atom_site_label_3 
 _geom_torsion_atom_site_label_4 
 _geom_torsion 
 _geom_torsion_site_symmetry_1 
 _geom_torsion_site_symmetry_2 
 _geom_torsion_site_symmetry_3 
 _geom_torsion_site_symmetry_4 
 _geom_torsion_publ_flag 
OW1 Ba B3 O1 173(6) . . . . ? 
O9 Ba B3 O1 103(6) 2_677 . . . ? 
O2 Ba B3 O1 34(6) 1_655 . . . ? 
O5 Ba B3 O1 39(6) . . . . ? 
O1 Ba B3 O1 48(6) 1_655 . . . ? 
O4 Ba B3 O1 -100(6) 1_545 . . . ? 
O6 Ba B3 O1 -84(6) . . . . ? 
O4 Ba B3 O1 -44(6) 2_676 . . . ? 
O3 Ba B3 O1 -118(6) 1_545 . . . ? 
O7 Ba B3 O1 157(6) . . . . ? 
B1 Ba B3 O1 41(6) 1_655 . . . ? 
OW1 Ba B3 O7 16.3(4) . . . . ? 
O9 Ba B3 O7 -53.9(3) 2_677 . . . ? 
O2 Ba B3 O7 -122.7(3) 1_655 . . . ? 
O5 Ba B3 O7 -117.3(5) . . . . ? 
O1 Ba B3 O7 -108.4(4) 1_655 . . . ? 
O4 Ba B3 O7 103.4(3) 1_545 . . . ? 
O6 Ba B3 O7 119.4(5) . . . . ? 
O4 Ba B3 O7 159.8(3) 2_676 . . . ? 
O3 Ba B3 O7 85.3(3) 1_545 . . . ? 
B1 Ba B3 O7 -115.6(3) 1_655 . . . ? 
OW1 Ba B3 O5 133.6(3) . . . . ? 
O9 Ba B3 O5 63.4(3) 2_677 . . . ? 
O2 Ba B3 O5 -5.4(3) 1_655 . . . ? 
O1 Ba B3 O5 8.9(5) 1_655 . . . ? 
O4 Ba B3 O5 -139.3(3) 1_545 . . . ? 
O6 Ba B3 O5 -123.3(5) . . . . ? 
O4 Ba B3 O5 -82.9(3) 2_676 . . . ? 
O3 Ba B3 O5 -157.4(3) 1_545 . . . ? 
O7 Ba B3 O5 117.3(5) . . . . ? 
B1 Ba B3 O5 1.7(4) 1_655 . . . ? 
OW1 Ba B3 O6 -103.1(3) . . . . ? 
O9 Ba B3 O6 -173.4(3) 2_677 . . . ? 
O2 Ba B3 O6 117.9(3) 1_655 . . . ? 
O5 Ba B3 O6 123.3(5) . . . . ? 
O1 Ba B3 O6 132.1(3) 1_655 . . . ? 
O4 Ba B3 O6 -16.0(4) 1_545 . . . ? 
O4 Ba B3 O6 40.3(3) 2_676 . . . ? 
O3 Ba B3 O6 -34.2(3) 1_545 . . . ? 
O7 Ba B3 O6 -119.4(5) . . . . ? 
B1 Ba B3 O6 125.0(3) 1_655 . . . ? 
O2 B1 O1 B3 165.9(6) . . . . ? 
O3 B1 O1 B3 -12.1(10) . . . . ? 
Ba B1 O1 B3 173.2(6) 1_455 . . . ? 
O2 B1 O1 Ba -7.3(6) . . . 1_455 ? 
O3 B1 O1 Ba 174.7(6) . . . 1_455 ? 
O7 B3 O1 B1 123.4(6) . . . . ? 
O5 B3 O1 B1 5.4(9) . . . . ? 
O6 B3 O1 B1 -115.0(6) . . . . ? 
Ba B3 O1 B1 -33(6) . . . . ? 
O7 B3 O1 Ba -67.9(8) . . . 1_455 ? 
O5 B3 O1 Ba 174.2(4) . . . 1_455 ? 
O6 B3 O1 Ba 53.8(8) . . . 1_455 ? 
Ba B3 O1 Ba 136(6) . . . 1_455 ? 
O1 B1 O2 Ga 160.0(5) . . . 2_576 ? 
O3 B1 O2 Ga -22.0(9) . . . 2_576 ? 
Ba B1 O2 Ga 152.4(5) 1_455 . . 2_576 ? 
O1 B1 O2 Ba 7.6(7) . . . 1_455 ? 
O3 B1 O2 Ba -174.4(5) . . . 1_455 ? 
O2 B1 O3 B2 -163.4(6) . . . . ? 
O1 B1 O3 B2 14.6(9) . . . . ? 
Ba B1 O3 B2 122(5) 1_455 . . . ? 
O2 B1 O3 Ba 45.2(11) . . . 1_565 ? 
O1 B1 O3 Ba -136.8(5) . . . 1_565 ? 
Ba B1 O3 Ba -30(6) 1_455 . . 1_565 ? 
O4 B2 O3 B1 165.6(6) . . . . ? 
O5 B2 O3 B1 -10.9(9) . . . . ? 
Ba B2 O3 B1 -163.9(6) 1_565 . . . ? 
Ba B2 O3 B1 111.1(5) 2_676 . . . ? 
O4 B2 O3 Ba -30.5(6) . . . 1_565 ? 
O5 B2 O3 Ba 153.0(6) . . . 1_565 ? 
Ba B2 O3 Ba -85.01(15) 2_676 . . 1_565 ? 
O5 B2 O4 Ga -15.4(10) . . . 2_676 ? 
O3 B2 O4 Ga 168.4(4) . . . 2_676 ? 
Ba B2 O4 Ga 137.1(5) 1_565 . . 2_676 ? 
Ba B2 O4 Ga -119.9(5) 2_676 . . 2_676 ? 
O5 B2 O4 Ba -152.5(6) . . . 1_565 ? 
O3 B2 O4 Ba 31.3(6) . . . 1_565 ? 
Ba B2 O4 Ba 103.05(18) 2_676 . . 1_565 ? 
O5 B2 O4 Ba 104.5(7) . . . 2_676 ? 
O3 B2 O4 Ba -71.8(5) . . . 2_676 ? 
Ba B2 O4 Ba -103.05(19) 1_565 . . 2_676 ? 
O4 B2 O5 B3 -171.4(6) . . . . ? 
O3 B2 O5 B3 4.7(10) . . . . ? 
Ba B2 O5 B3 93.9(13) 1_565 . . . ? 
Ba B2 O5 B3 -101.2(6) 2_676 . . . ? 
O4 B2 O5 Ba -0.3(13) . . . . ? 
O3 B2 O5 Ba 175.8(4) . . . . ? 
Ba B2 O5 Ba -95.0(13) 1_565 . . . ? 
Ba B2 O5 Ba 69.9(9) 2_676 . . . ? 
O1 B3 O5 B2 -1.8(9) . . . . ? 
O7 B3 O5 B2 -122.0(6) . . . . ? 
O6 B3 O5 B2 120.5(6) . . . . ? 
Ba B3 O5 B2 175.3(6) . . . . ? 
O1 B3 O5 Ba -177.1(5) . . . . ? 
O7 B3 O5 Ba 62.7(4) . . . . ? 
O6 B3 O5 Ba -54.8(4) . . . . ? 
OW1 Ba O5 B2 129.2(8) . . . . ? 
O9 Ba O5 B2 75.3(8) 2_677 . . . ? 
O2 Ba O5 B2 1.7(8) 1_655 . . . ? 
O1 Ba O5 B2 13.0(8) 1_655 . . . ? 
O4 Ba O5 B2 -97.2(8) 1_545 . . . ? 
O6 Ba O5 B2 -141.3(8) . . . . ? 
O4 Ba O5 B2 -82.5(8) 2_676 . . . ? 
O3 Ba O5 B2 -146.7(8) 1_545 . . . ? 
O7 Ba O5 B2 153.3(9) . . . . ? 
B3 Ba O5 B2 -172.6(10) . . . . ? 
B1 Ba O5 B2 8.9(8) 1_655 . . . ? 
OW1 Ba O5 B3 -58.2(4) . . . . ? 
O9 Ba O5 B3 -112.1(4) 2_677 . . . ? 
O2 Ba O5 B3 174.3(4) 1_655 . . . ? 
O1 Ba O5 B3 -174.3(3) 1_655 . . . ? 
O4 Ba O5 B3 75.4(4) 1_545 . . . ? 
O6 Ba O5 B3 31.3(3) . . . . ? 
O4 Ba O5 B3 90.1(3) 2_676 . . . ? 
O3 Ba O5 B3 25.9(4) 1_545 . . . ? 
O7 Ba O5 B3 -34.1(3) . . . . ? 
B1 Ba O5 B3 -178.5(4) 1_655 . . . ? 
O1 B3 O6 Ga -64.4(6) . . . 2_566 ? 
O7 B3 O6 Ga 57.4(7) . . . 2_566 ? 
O5 B3 O6 Ga 172.5(3) . . . 2_566 ? 
Ba B3 O6 Ga 120.2(3) . . . 2_566 ? 
O1 B3 O6 Ga 73.7(7) . . . . ? 
O7 B3 O6 Ga -164.5(4) . . . . ? 
O5 B3 O6 Ga -49.4(7) . . . . ? 
Ba B3 O6 Ga -101.7(4) . . . . ? 
O1 B3 O6 Ba 175.4(5) . . . . ? 
O7 B3 O6 Ba -62.8(5) . . . . ? 
O5 B3 O6 Ba 52.3(4) . . . . ? 
O2 Ga O6 B3 -16.0(5) 2_576 . . . ? 
O4 Ga O6 B3 98.5(5) 2_676 . . . ? 
O6 Ga O6 B3 -144.0(6) 2_566 . . . ? 
O8 Ga O6 B3 -133.7(12) 2_566 . . . ? 
O2 Ga O6 Ga 127.9(2) 2_576 . . 2_566 ? 
O4 Ga O6 Ga -117.5(2) 2_676 . . 2_566 ? 
O6 Ga O6 Ga 0.0 2_566 . . 2_566 ? 
O8 Ga O6 Ga 10.3(14) 2_566 . . 2_566 ? 
O2 Ga O6 Ba -107.83(18) 2_576 . . . ? 
O4 Ga O6 Ba 6.73(16) 2_676 . . . ? 
O6 Ga O6 Ba 124.2(2) 2_566 . . . ? 
O8 Ga O6 Ba 134.5(13) 2_566 . . . ? 
OW1 Ba O6 B3 87.6(3) . . . . ? 
O9 Ba O6 B3 7.2(4) 2_677 . . . ? 
O2 Ba O6 B3 -68.4(3) 1_655 . . . ? 
O5 Ba O6 B3 -31.5(3) . . . . ? 
O1 Ba O6 B3 -96.7(4) 1_655 . . . ? 
O4 Ba O6 B3 168.4(3) 1_545 . . . ? 
O4 Ba O6 B3 -131.3(3) 2_676 . . . ? 
O3 Ba O6 B3 143.4(3) 1_545 . . . ? 
O7 Ba O6 B3 33.1(3) . . . . ? 
B1 Ba O6 B3 -74.7(4) 1_655 . . . ? 
OW1 Ba O6 Ga -34.0(3) . . . 2_566 ? 
O9 Ba O6 Ga -114.3(2) 2_677 . . 2_566 ? 
O2 Ba O6 Ga 170.10(19) 1_655 . . 2_566 ? 
O5 Ba O6 Ga -153.1(3) . . . 2_566 ? 
O1 Ba O6 Ga 141.7(2) 1_655 . . 2_566 ? 
O4 Ba O6 Ga 46.9(2) 1_545 . . 2_566 ? 
O4 Ba O6 Ga 107.2(2) 2_676 . . 2_566 ? 
O3 Ba O6 Ga 21.88(19) 1_545 . . 2_566 ? 
O7 Ba O6 Ga -88.5(2) . . . 2_566 ? 
B3 Ba O6 Ga -121.5(4) . . . 2_566 ? 
B1 Ba O6 Ga 163.8(2) 1_655 . . 2_566 ? 
OW1 Ba O6 Ga -146.29(17) . . . . ? 
O9 Ba O6 Ga 133.37(15) 2_677 . . . ? 
O2 Ba O6 Ga 57.78(18) 1_655 . . . ? 
O5 Ba O6 Ga 94.62(19) . . . . ? 
O1 Ba O6 Ga 29.4(3) 1_655 . . . ? 
O4 Ba O6 Ga -65.45(17) 1_545 . . . ? 
O4 Ba O6 Ga -5.12(12) 2_676 . . . ? 
O3 Ba O6 Ga -90.44(16) 1_545 . . . ? 
O7 Ba O6 Ga 159.2(2) . . . . ? 
B3 Ba O6 Ga 126.1(4) . . . . ? 
B1 Ba O6 Ga 51.4(3) 1_655 . . . ? 
O8 B4 O7 B3 12.5(11) . . . . ? 
O9 B4 O7 B3 -167.5(6) . . . . ? 
O8 B4 O7 Ba -76.6(8) . . . . ? 
O9 B4 O7 Ba 103.4(6) . . . . ? 
O1 B3 O7 B4 76.5(7) . . . . ? 
O5 B3 O7 B4 -161.8(6) . . . . ? 
O6 B3 O7 B4 -45.8(9) . . . . ? 
Ba B3 O7 B4 -105.3(6) . . . . ? 
O1 B3 O7 Ba -178.2(5) . . . . ? 
O5 B3 O7 Ba -56.5(4) . . . . ? 
O6 B3 O7 Ba 59.5(5) . . . . ? 
OW1 Ba O7 B4 -41.4(5) . . . . ? 
O9 Ba O7 B4 -115.6(5) 2_677 . . . ? 
O2 Ba O7 B4 -173.3(4) 1_655 . . . ? 
O5 Ba O7 B4 158.0(5) . . . . ? 
O1 Ba O7 B4 -124.6(4) 1_655 . . . ? 
O4 Ba O7 B4 16.8(5) 1_545 . . . ? 
O6 Ba O7 B4 89.4(5) . . . . ? 
O4 Ba O7 B4 102.8(4) 2_676 . . . ? 
O3 Ba O7 B4 27.5(5) 1_545 . . . ? 
B3 Ba O7 B4 123.1(6) . . . . ? 
B1 Ba O7 B4 -153.6(4) 1_655 . . . ? 
OW1 Ba O7 B3 -164.5(4) . . . . ? 
O9 Ba O7 B3 121.3(3) 2_677 . . . ? 
O2 Ba O7 B3 63.6(3) 1_655 . . . ? 
O5 Ba O7 B3 34.9(3) . . . . ? 
O1 Ba O7 B3 112.3(4) 1_655 . . . ? 
O4 Ba O7 B3 -106.3(3) 1_545 . . . ? 
O6 Ba O7 B3 -33.7(3) . . . . ? 
O4 Ba O7 B3 -20.3(3) 2_676 . . . ? 
O3 Ba O7 B3 -95.6(3) 1_545 . . . ? 
B1 Ba O7 B3 83.3(4) 1_655 . . . ? 
O9 B4 O8 Ga -170.2(5) . . . 2_566 ? 
O7 B4 O8 Ga 9.8(11) . . . 2_566 ? 
O8 B4 O9 Ba -159.4(5) . . . 2_677 ? 
O7 B4 O9 Ba 20.6(11) . . . 2_677 ? 
 
loop_ 
 _geom_hbond_atom_site_label_D 
 _geom_hbond_atom_site_label_H 
 _geom_hbond_atom_site_label_A 
 _geom_hbond_distance_DH 
 _geom_hbond_distance_HA 
 _geom_hbond_distance_DA 
 _geom_hbond_angle_DHA 
 _geom_hbond_site_symmetry_A 
OW1 H1B O8  0.90 2.48 3.226(11) 140.1 1_655 
O9 H9A O8  0.82 1.90 2.705(6) 168.6 2_567 
 
_diffrn_measured_fraction_theta_max    0.967 
_diffrn_reflns_theta_full              27.54 
_diffrn_measured_fraction_theta_full   0.967 
_refine_diff_density_max    1.137 
_refine_diff_density_min   -1.255 
_refine_diff_density_rms    0.315 

